# Electronic Supplementary Material (ESI) for Dalton Transactions.
# This journal is © The Royal Society of Chemistry 2019

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_I
_database_code_depnum_ccdc_archive 'CCDC 1892328'
loop_
_audit_author_name
_audit_author_address
'Igor Plokhikh'
;University of Regensburg
Germany
;
_audit_update_record             
;
2019-01-21 deposited with the CCDC.	2019-09-23 downloaded from the CCDC.
;
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        'europium platinum phosphide'
_chemical_name_common            'europium platinum phosphide'
_chemical_formula_moiety         'Eu Pt3 P'
_chemical_formula_sum            'Eu Pt3 P'
_chemical_compound_source        'solid state reaction'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_weight         768.2
_chemical_melting_point          ?
_exptl_crystal_colour            black

_diffrn_ambient_temperature      293
_diffrn_ambient_pressure         101.3

#=======================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_H-M   'P 4/n m m'
_symmetry_Int_Tables_number      129
_chemical_absolute_configuration .
_symmetry_space_group_name_Hall  '-P 4a;-2a'

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x,-y,z
3 -y+1/2,x+1/2,z
4 y+1/2,-x+1/2,z
5 -x+1/2,y+1/2,-z
6 x+1/2,-y+1/2,-z
7 y,x,-z
8 -y,-x,-z
9 -x+1/2,-y+1/2,-z
10 x+1/2,y+1/2,-z
11 y,-x,-z
12 -y,x,-z
13 x,-y,z
14 -x,y,z
15 -y+1/2,-x+1/2,z
16 y+1/2,x+1/2,z

_cell_length_a                   5.74507(8)
_cell_length_b                   5.74507(8)
_cell_length_c                   5.42138(11)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     178.937(5)


_cell_formula_units_Z            2
_cell_measurement_temperature    293
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    14.2573
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             432

_pd_spec_size_axial              ?
_pd_spec_size_equat              ?
_pd_spec_size_thick              ?
_pd_spec_mounting                ?
_pd_spec_mount_mode              ?
_pd_spec_shape                   ?
_pd_char_particle_morphology     ?
_pd_char_colour                  ?
_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

_exptl_absorpt_coefficient_mu    135.107
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?
_pd_instr_location               
; ?
;
_pd_calibration_special_details  
; ?
;

_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7093
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_type              'STOE STADI P'
_diffrn_source_target            ?
_diffrn_radiation_monochromator  ?
_diffrn_measurement_device       'powder diffractometer'
_diffrn_measurement_device_type  'powder diffractometer'
_diffrn_detector                 ?
_diffrn_detector_type            ?

_pd_meas_scan_method             ?
_pd_meas_special_details         
; ?
;
_pd_meas_number_of_points        4329
_pd_meas_2theta_range_min        6.005
_pd_meas_2theta_range_max        70.925
_pd_meas_2theta_range_inc        0.015

#=======================================================================

# 8. REFINEMENT DATA

_pd_proc_ls_special_details      
; ?
;
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_background_function  '20 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_prof_R_factor        0.0193
_pd_proc_ls_prof_wR_factor       0.0267
_pd_proc_ls_prof_wR_expected     0.0136

_refine_special_details          
; ?
;

_refine_ls_R_factor_gt           0.0340
_refine_ls_wR_factor_gt          0.0322
_refine_ls_R_factor_all          0.0361
_refine_ls_wR_factor_all         0.0326
_refine_ls_goodness_of_fit_all   1.97
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_parameters     44
_refine_ls_number_restraints     1
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0363
_refine_ls_shift/su_mean         0.0067
_refine_diff_density_max         2.98
_refine_diff_density_min         -2.62
_refine_ls_extinction_method     ?
_refine_ls_extinction_coef       ?
_refine_ls_extinction_expression ?

_pd_proc_2theta_range_min        6.005
_pd_proc_2theta_range_max        70.925
_pd_proc_2theta_range_inc        0.015
_pd_proc_wavelength              ?

_pd_block_diffractogram_id       ?

loop_
_pd_proc_info_excluded_regions
'from 0 to 6.000'
_pd_proc_info_data_reduction     ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu -0.1003 3.6972 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
P 0.1037 0.0957 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Pt -1.6632 8.4516 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0 0.5 0.1451(3) Uani 0.0043(4) 2 1 d . . .
Pt2 Pt 0.25 0.25 -0.5 Uani 0.0068(3) 4 1 d . . .
Eu2 Eu 0 1 0 Uiso 0.0056(6) 2 1 d . . .
P1 P 0 0.5 -0.2789(10) Uiso 0.028(4) 2 1 d . . .


loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Pt1 Pt2 . 1_556 2.7977(10) ?
Pt1 Pt2 . 2_566 2.7977(10) ?
Pt1 Pt2 . 3_556 2.7977(10) ?
Pt1 Pt2 . 4_456 2.7977(10) ?
Pt1 Eu2 . 1_545 2.9783(4) ?
Pt1 Eu2 . . 2.9783(4) ?
Pt1 Eu2 . 3_555 2.9783(4) ?
Pt1 Eu2 . 3_655 2.9783(4) ?
Pt1 P1 . . 2.299(6) ?
Pt1 P1 . 1_556 3.123(6) ?
Pt2 Pt2 . 3_545 2.87253(8) ?
Pt2 Pt2 . 3_555 2.87253(8) ?
Pt2 Pt2 . 4_455 2.87253(8) ?
Pt2 Pt2 . 4_555 2.87253(8) ?
Pt2 Eu2 . 1_544 3.38727(9) ?
Pt2 Eu2 . 1_545 3.38727(9) ?
Pt2 Eu2 . 3_654 3.38727(9) ?
Pt2 Eu2 . 3_655 3.38727(9) ?
Pt2 P1 . . 2.359(3) ?
Pt2 P1 . 5_544 2.359(3) ?
Eu2 Eu2 . 3_555 4.06238(8) ?
Eu2 Eu2 . 3_565 4.06238(8) ?
Eu2 Eu2 . 3_655 4.06238(8) ?
Eu2 Eu2 . 3_665 4.06238(8) ?
Eu2 P1 . . 3.246(3) ?
Eu2 P1 . 1_565 3.246(3) ?
Eu2 P1 . 5_455 3.246(3) ?
Eu2 P1 . 5_555 3.246(3) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Pt2 Pt1 Pt2 1_556 . 2_566 93.11(4) ?
Pt2 Pt1 Pt2 1_556 . 3_556 61.78(2) ?
Pt2 Pt1 Pt2 1_556 . 4_456 61.78(2) ?
Pt2 Pt1 Eu2 1_556 . 1_545 71.731(8) ?
Pt2 Pt1 Eu2 1_556 . . 132.59(3) ?
Pt2 Pt1 Eu2 1_556 . 3_555 132.59(3) ?
Pt2 Pt1 Eu2 1_556 . 3_655 71.731(8) ?
Pt2 Pt1 P1 1_556 . . 133.45(2) ?
Pt2 Pt1 P1 1_556 . 1_556 46.55(2) ?
Pt2 Pt1 Pt2 2_566 . 3_556 61.78(2) ?
Pt2 Pt1 Pt2 2_566 . 4_456 61.78(2) ?
Pt2 Pt1 Eu2 2_566 . 1_545 132.59(3) ?
Pt2 Pt1 Eu2 2_566 . . 71.731(8) ?
Pt2 Pt1 Eu2 2_566 . 3_555 71.731(8) ?
Pt2 Pt1 Eu2 2_566 . 3_655 132.59(3) ?
Pt2 Pt1 P1 2_566 . . 133.45(2) ?
Pt2 Pt1 P1 2_566 . 1_556 46.55(2) ?
Pt2 Pt1 Pt2 3_556 . 4_456 93.11(4) ?
Pt2 Pt1 Eu2 3_556 . 1_545 132.59(3) ?
Pt2 Pt1 Eu2 3_556 . . 71.731(8) ?
Pt2 Pt1 Eu2 3_556 . 3_555 132.59(3) ?
Pt2 Pt1 Eu2 3_556 . 3_655 71.731(8) ?
Pt2 Pt1 P1 3_556 . . 133.45(2) ?
Pt2 Pt1 P1 3_556 . 1_556 46.55(2) ?
Pt2 Pt1 Eu2 4_456 . 1_545 71.731(8) ?
Pt2 Pt1 Eu2 4_456 . . 132.59(3) ?
Pt2 Pt1 Eu2 4_456 . 3_555 71.731(8) ?
Pt2 Pt1 Eu2 4_456 . 3_655 132.59(3) ?
Pt2 Pt1 P1 4_456 . . 133.45(2) ?
Pt2 Pt1 P1 4_456 . 1_556 46.55(2) ?
Eu2 Pt1 Eu2 1_545 . . 149.37(5) ?
Eu2 Pt1 Eu2 1_545 . 3_555 85.999(14) ?
Eu2 Pt1 Eu2 1_545 . 3_655 85.999(14) ?
Eu2 Pt1 P1 1_545 . . 74.68(3) ?
Eu2 Pt1 P1 1_545 . 1_556 105.32(3) ?
Eu2 Pt1 Eu2 . . 3_555 85.999(14) ?
Eu2 Pt1 Eu2 . . 3_655 85.999(14) ?
Eu2 Pt1 P1 . . . 74.68(3) ?
Eu2 Pt1 P1 . . 1_556 105.32(3) ?
Eu2 Pt1 Eu2 3_555 . 3_655 149.37(5) ?
Eu2 Pt1 P1 3_555 . . 74.68(3) ?
Eu2 Pt1 P1 3_555 . 1_556 105.32(3) ?
Eu2 Pt1 P1 3_655 . . 74.68(3) ?
Eu2 Pt1 P1 3_655 . 1_556 105.32(3) ?
P1 Pt1 P1 . . 1_556 180 ?
Pt1 Pt2 Pt1 1_554 . 5_545 180 ?
Pt1 Pt2 Pt2 1_554 . 3_545 120.888(12) ?
Pt1 Pt2 Pt2 1_554 . 3_555 59.112(12) ?
Pt1 Pt2 Pt2 1_554 . 4_455 59.112(12) ?
Pt1 Pt2 Pt2 1_554 . 4_555 120.888(12) ?
Pt1 Pt2 Eu2 1_554 . 1_544 56.611(15) ?
Pt1 Pt2 Eu2 1_554 . 1_545 123.389(15) ?
Pt1 Pt2 Eu2 1_554 . 3_654 56.611(15) ?
Pt1 Pt2 Eu2 1_554 . 3_655 123.389(15) ?
Pt1 Pt2 P1 1_554 . . 74.00(12) ?
Pt1 Pt2 P1 1_554 . 5_544 106.00(12) ?
Pt1 Pt2 Pt2 5_545 . 3_545 59.112(12) ?
Pt1 Pt2 Pt2 5_545 . 3_555 120.888(12) ?
Pt1 Pt2 Pt2 5_545 . 4_455 120.888(12) ?
Pt1 Pt2 Pt2 5_545 . 4_555 59.112(12) ?
Pt1 Pt2 Eu2 5_545 . 1_544 123.389(15) ?
Pt1 Pt2 Eu2 5_545 . 1_545 56.611(15) ?
Pt1 Pt2 Eu2 5_545 . 3_654 123.389(15) ?
Pt1 Pt2 Eu2 5_545 . 3_655 56.611(15) ?
Pt1 Pt2 P1 5_545 . . 106.00(12) ?
Pt1 Pt2 P1 5_545 . 5_544 74.00(12) ?
Pt2 Pt2 Pt2 3_545 . 3_555 180 ?
Pt2 Pt2 Pt2 3_545 . 4_455 90 ?
Pt2 Pt2 Pt2 3_545 . 4_555 90 ?
Pt2 Pt2 Eu2 3_545 . 1_544 64.9114(5) ?
Pt2 Pt2 Eu2 3_545 . 1_545 64.9114(5) ?
Pt2 Pt2 Eu2 3_545 . 3_654 115.0886(5) ?
Pt2 Pt2 Eu2 3_545 . 3_655 115.0886(5) ?
Pt2 Pt2 P1 3_545 . . 127.51(5) ?
Pt2 Pt2 P1 3_545 . 5_544 52.49(5) ?
Pt2 Pt2 Pt2 3_555 . 4_455 90 ?
Pt2 Pt2 Pt2 3_555 . 4_555 90 ?
Pt2 Pt2 Eu2 3_555 . 1_544 115.0886(5) ?
Pt2 Pt2 Eu2 3_555 . 1_545 115.0886(5) ?
Pt2 Pt2 Eu2 3_555 . 3_654 64.9114(5) ?
Pt2 Pt2 Eu2 3_555 . 3_655 64.9114(5) ?
Pt2 Pt2 P1 3_555 . . 52.49(5) ?
Pt2 Pt2 P1 3_555 . 5_544 127.51(5) ?
Pt2 Pt2 Pt2 4_455 . 4_555 180 ?
Pt2 Pt2 Eu2 4_455 . 1_544 64.9114(5) ?
Pt2 Pt2 Eu2 4_455 . 1_545 64.9114(5) ?
Pt2 Pt2 Eu2 4_455 . 3_654 115.0886(5) ?
Pt2 Pt2 Eu2 4_455 . 3_655 115.0886(5) ?
Pt2 Pt2 P1 4_455 . . 52.49(5) ?
Pt2 Pt2 P1 4_455 . 5_544 127.51(5) ?
Pt2 Pt2 Eu2 4_555 . 1_544 115.0886(5) ?
Pt2 Pt2 Eu2 4_555 . 1_545 115.0886(5) ?
Pt2 Pt2 Eu2 4_555 . 3_654 64.9114(5) ?
Pt2 Pt2 Eu2 4_555 . 3_655 64.9114(5) ?
Pt2 Pt2 P1 4_555 . . 127.51(5) ?
Pt2 Pt2 P1 4_555 . 5_544 52.49(5) ?
Eu2 Pt2 Eu2 1_544 . 1_545 106.3097(12) ?
Eu2 Pt2 Eu2 1_544 . 3_654 73.6903(12) ?
Eu2 Pt2 Eu2 1_544 . 3_655 180 ?
Eu2 Pt2 P1 1_544 . . 114.00(9) ?
Eu2 Pt2 P1 1_544 . 5_544 66.00(9) ?
Eu2 Pt2 Eu2 1_545 . 3_654 180 ?
Eu2 Pt2 Eu2 1_545 . 3_655 73.6903(12) ?
Eu2 Pt2 P1 1_545 . . 66.00(9) ?
Eu2 Pt2 P1 1_545 . 5_544 114.00(9) ?
Eu2 Pt2 Eu2 3_654 . 3_655 106.3097(12) ?
Eu2 Pt2 P1 3_654 . . 114.00(9) ?
Eu2 Pt2 P1 3_654 . 5_544 66.00(9) ?
Eu2 Pt2 P1 3_655 . . 66.00(9) ?
Eu2 Pt2 P1 3_655 . 5_544 114.00(9) ?
P1 Pt2 P1 . . 5_544 180 ?
Pt1 Eu2 Pt1 . . 1_565 149.37(4) ?
Pt1 Eu2 Pt1 . . 5_455 94.001(10) ?
Pt1 Eu2 Pt1 . . 5_555 94.001(10) ?
Pt1 Eu2 Pt2 . . 1_565 128.34(2) ?
Pt1 Eu2 Pt2 . . 1_566 101.39(2) ?
Pt1 Eu2 Pt2 . . 2_565 78.61(2) ?
Pt1 Eu2 Pt2 . . 2_566 51.66(2) ?
Pt1 Eu2 Pt2 . . 3_555 78.61(2) ?
Pt1 Eu2 Pt2 . . 3_556 51.66(2) ?
Pt1 Eu2 Pt2 . . 4_465 128.34(2) ?
Pt1 Eu2 Pt2 . . 4_466 101.39(2) ?
Pt1 Eu2 Eu2 . . 3_555 47.001(7) ?
Pt1 Eu2 Eu2 . . 3_565 132.999(7) ?
Pt1 Eu2 Eu2 . . 3_655 47.001(7) ?
Pt1 Eu2 Eu2 . . 3_665 132.999(7) ?
Pt1 Eu2 P1 . . . 43.08(9) ?
Pt1 Eu2 P1 . . 1_565 167.56(9) ?
Pt1 Eu2 P1 . . 5_455 82.93(2) ?
Pt1 Eu2 P1 . . 5_555 82.93(2) ?
Pt1 Eu2 Pt1 1_565 . 5_455 94.001(10) ?
Pt1 Eu2 Pt1 1_565 . 5_555 94.001(10) ?
Pt1 Eu2 Pt2 1_565 . 1_565 78.61(2) ?
Pt1 Eu2 Pt2 1_565 . 1_566 51.66(2) ?
Pt1 Eu2 Pt2 1_565 . 2_565 128.34(2) ?
Pt1 Eu2 Pt2 1_565 . 2_566 101.39(2) ?
Pt1 Eu2 Pt2 1_565 . 3_555 128.34(2) ?
Pt1 Eu2 Pt2 1_565 . 3_556 101.39(2) ?
Pt1 Eu2 Pt2 1_565 . 4_465 78.61(2) ?
Pt1 Eu2 Pt2 1_565 . 4_466 51.66(2) ?
Pt1 Eu2 Eu2 1_565 . 3_555 132.999(7) ?
Pt1 Eu2 Eu2 1_565 . 3_565 47.001(7) ?
Pt1 Eu2 Eu2 1_565 . 3_655 132.999(7) ?
Pt1 Eu2 Eu2 1_565 . 3_665 47.001(7) ?
Pt1 Eu2 P1 1_565 . . 167.56(9) ?
Pt1 Eu2 P1 1_565 . 1_565 43.08(9) ?
Pt1 Eu2 P1 1_565 . 5_455 82.93(2) ?
Pt1 Eu2 P1 1_565 . 5_555 82.93(2) ?
Pt1 Eu2 Pt1 5_455 . 5_555 149.37(4) ?
Pt1 Eu2 Pt2 5_455 . 1_565 101.39(2) ?
Pt1 Eu2 Pt2 5_455 . 1_566 128.34(2) ?
Pt1 Eu2 Pt2 5_455 . 2_565 51.66(2) ?
Pt1 Eu2 Pt2 5_455 . 2_566 78.61(2) ?
Pt1 Eu2 Pt2 5_455 . 3_555 101.39(2) ?
Pt1 Eu2 Pt2 5_455 . 3_556 128.34(2) ?
Pt1 Eu2 Pt2 5_455 . 4_465 51.66(2) ?
Pt1 Eu2 Pt2 5_455 . 4_466 78.61(2) ?
Pt1 Eu2 Eu2 5_455 . 3_555 47.001(7) ?
Pt1 Eu2 Eu2 5_455 . 3_565 47.001(7) ?
Pt1 Eu2 Eu2 5_455 . 3_655 132.999(7) ?
Pt1 Eu2 Eu2 5_455 . 3_665 132.999(7) ?
Pt1 Eu2 P1 5_455 . . 82.93(2) ?
Pt1 Eu2 P1 5_455 . 1_565 82.93(2) ?
Pt1 Eu2 P1 5_455 . 5_455 43.08(9) ?
Pt1 Eu2 P1 5_455 . 5_555 167.56(9) ?
Pt1 Eu2 Pt2 5_555 . 1_565 51.66(2) ?
Pt1 Eu2 Pt2 5_555 . 1_566 78.61(2) ?
Pt1 Eu2 Pt2 5_555 . 2_565 101.39(2) ?
Pt1 Eu2 Pt2 5_555 . 2_566 128.34(2) ?
Pt1 Eu2 Pt2 5_555 . 3_555 51.66(2) ?
Pt1 Eu2 Pt2 5_555 . 3_556 78.61(2) ?
Pt1 Eu2 Pt2 5_555 . 4_465 101.39(2) ?
Pt1 Eu2 Pt2 5_555 . 4_466 128.34(2) ?
Pt1 Eu2 Eu2 5_555 . 3_555 132.999(7) ?
Pt1 Eu2 Eu2 5_555 . 3_565 132.999(7) ?
Pt1 Eu2 Eu2 5_555 . 3_655 47.001(7) ?
Pt1 Eu2 Eu2 5_555 . 3_665 47.001(7) ?
Pt1 Eu2 P1 5_555 . . 82.93(2) ?
Pt1 Eu2 P1 5_555 . 1_565 82.93(2) ?
Pt1 Eu2 P1 5_555 . 5_455 167.56(9) ?
Pt1 Eu2 P1 5_555 . 5_555 43.08(9) ?
Pt2 Eu2 Pt2 1_565 . 1_566 106.3097(12) ?
Pt2 Eu2 Pt2 1_565 . 2_565 73.6903(12) ?
Pt2 Eu2 Pt2 1_565 . 2_566 180 ?
Pt2 Eu2 Pt2 1_565 . 3_555 50.1773(9) ?
Pt2 Eu2 Pt2 1_565 . 3_556 129.8227(9) ?
Pt2 Eu2 Pt2 1_565 . 4_465 50.1773(9) ?
Pt2 Eu2 Pt2 1_565 . 4_466 129.8227(9) ?
Pt2 Eu2 Eu2 1_565 . 3_555 126.8452(6) ?
Pt2 Eu2 Eu2 1_565 . 3_565 90.0000(7) ?
Pt2 Eu2 Eu2 1_565 . 3_655 90.0000(7) ?
Pt2 Eu2 Eu2 1_565 . 3_665 53.1548(6) ?
Pt2 Eu2 P1 1_565 . . 90.14(8) ?
Pt2 Eu2 P1 1_565 . 1_565 41.59(7) ?
Pt2 Eu2 P1 1_565 . 5_455 138.41(7) ?
Pt2 Eu2 P1 1_565 . 5_555 89.86(8) ?
Pt2 Eu2 Pt2 1_566 . 2_565 180 ?
Pt2 Eu2 Pt2 1_566 . 2_566 73.6903(12) ?
Pt2 Eu2 Pt2 1_566 . 3_555 129.8227(9) ?
Pt2 Eu2 Pt2 1_566 . 3_556 50.1773(9) ?
Pt2 Eu2 Pt2 1_566 . 4_465 129.8227(9) ?
Pt2 Eu2 Pt2 1_566 . 4_466 50.1773(9) ?
Pt2 Eu2 Eu2 1_566 . 3_555 126.8452(6) ?
Pt2 Eu2 Eu2 1_566 . 3_565 90.0000(7) ?
Pt2 Eu2 Eu2 1_566 . 3_655 90.0000(7) ?
Pt2 Eu2 Eu2 1_566 . 3_665 53.1548(6) ?
Pt2 Eu2 P1 1_566 . . 138.41(7) ?
Pt2 Eu2 P1 1_566 . 1_565 89.86(8) ?
Pt2 Eu2 P1 1_566 . 5_455 90.14(8) ?
Pt2 Eu2 P1 1_566 . 5_555 41.59(7) ?
Pt2 Eu2 Pt2 2_565 . 2_566 106.3097(12) ?
Pt2 Eu2 Pt2 2_565 . 3_555 50.1773(9) ?
Pt2 Eu2 Pt2 2_565 . 3_556 129.8227(9) ?
Pt2 Eu2 Pt2 2_565 . 4_465 50.1773(9) ?
Pt2 Eu2 Pt2 2_565 . 4_466 129.8227(9) ?
Pt2 Eu2 Eu2 2_565 . 3_555 53.1548(6) ?
Pt2 Eu2 Eu2 2_565 . 3_565 90.0000(7) ?
Pt2 Eu2 Eu2 2_565 . 3_655 90.0000(7) ?
Pt2 Eu2 Eu2 2_565 . 3_665 126.8452(6) ?
Pt2 Eu2 P1 2_565 . . 41.59(7) ?
Pt2 Eu2 P1 2_565 . 1_565 90.14(8) ?
Pt2 Eu2 P1 2_565 . 5_455 89.86(8) ?
Pt2 Eu2 P1 2_565 . 5_555 138.41(7) ?
Pt2 Eu2 Pt2 2_566 . 3_555 129.8227(9) ?
Pt2 Eu2 Pt2 2_566 . 3_556 50.1773(9) ?
Pt2 Eu2 Pt2 2_566 . 4_465 129.8227(9) ?
Pt2 Eu2 Pt2 2_566 . 4_466 50.1773(9) ?
Pt2 Eu2 Eu2 2_566 . 3_555 53.1548(6) ?
Pt2 Eu2 Eu2 2_566 . 3_565 90.0000(7) ?
Pt2 Eu2 Eu2 2_566 . 3_655 90.0000(7) ?
Pt2 Eu2 Eu2 2_566 . 3_665 126.8452(6) ?
Pt2 Eu2 P1 2_566 . . 89.86(8) ?
Pt2 Eu2 P1 2_566 . 1_565 138.41(7) ?
Pt2 Eu2 P1 2_566 . 5_455 41.59(7) ?
Pt2 Eu2 P1 2_566 . 5_555 90.14(8) ?
Pt2 Eu2 Pt2 3_555 . 3_556 106.3097(12) ?
Pt2 Eu2 Pt2 3_555 . 4_465 73.6903(12) ?
Pt2 Eu2 Pt2 3_555 . 4_466 180 ?
Pt2 Eu2 Eu2 3_555 . 3_555 90.0000(7) ?
Pt2 Eu2 Eu2 3_555 . 3_565 126.8452(6) ?
Pt2 Eu2 Eu2 3_555 . 3_655 53.1548(6) ?
Pt2 Eu2 Eu2 3_555 . 3_665 90.0000(7) ?
Pt2 Eu2 P1 3_555 . . 41.59(7) ?
Pt2 Eu2 P1 3_555 . 1_565 90.14(8) ?
Pt2 Eu2 P1 3_555 . 5_455 138.41(7) ?
Pt2 Eu2 P1 3_555 . 5_555 89.86(8) ?
Pt2 Eu2 Pt2 3_556 . 4_465 180 ?
Pt2 Eu2 Pt2 3_556 . 4_466 73.6903(12) ?
Pt2 Eu2 Eu2 3_556 . 3_555 90.0000(7) ?
Pt2 Eu2 Eu2 3_556 . 3_565 126.8452(6) ?
Pt2 Eu2 Eu2 3_556 . 3_655 53.1548(6) ?
Pt2 Eu2 Eu2 3_556 . 3_665 90.0000(7) ?
Pt2 Eu2 P1 3_556 . . 89.86(8) ?
Pt2 Eu2 P1 3_556 . 1_565 138.41(7) ?
Pt2 Eu2 P1 3_556 . 5_455 90.14(8) ?
Pt2 Eu2 P1 3_556 . 5_555 41.59(7) ?
Pt2 Eu2 Pt2 4_465 . 4_466 106.3097(12) ?
Pt2 Eu2 Eu2 4_465 . 3_555 90.0000(7) ?
Pt2 Eu2 Eu2 4_465 . 3_565 53.1548(6) ?
Pt2 Eu2 Eu2 4_465 . 3_655 126.8452(6) ?
Pt2 Eu2 Eu2 4_465 . 3_665 90.0000(7) ?
Pt2 Eu2 P1 4_465 . . 90.14(8) ?
Pt2 Eu2 P1 4_465 . 1_565 41.59(7) ?
Pt2 Eu2 P1 4_465 . 5_455 89.86(8) ?
Pt2 Eu2 P1 4_465 . 5_555 138.41(7) ?
Pt2 Eu2 Eu2 4_466 . 3_555 90.0000(7) ?
Pt2 Eu2 Eu2 4_466 . 3_565 53.1548(6) ?
Pt2 Eu2 Eu2 4_466 . 3_655 126.8452(6) ?
Pt2 Eu2 Eu2 4_466 . 3_665 90.0000(7) ?
Pt2 Eu2 P1 4_466 . . 138.41(7) ?
Pt2 Eu2 P1 4_466 . 1_565 89.86(8) ?
Pt2 Eu2 P1 4_466 . 5_455 41.59(7) ?
Pt2 Eu2 P1 4_466 . 5_555 90.14(8) ?
Eu2 Eu2 Eu2 3_555 . 3_565 90.0000(11) ?
Eu2 Eu2 Eu2 3_555 . 3_655 90.0000(11) ?
Eu2 Eu2 Eu2 3_555 . 3_665 180 ?
Eu2 Eu2 P1 3_555 . . 51.26(4) ?
Eu2 Eu2 P1 3_555 . 1_565 128.74(4) ?
Eu2 Eu2 P1 3_555 . 5_455 51.26(4) ?
Eu2 Eu2 P1 3_555 . 5_555 128.74(4) ?
Eu2 Eu2 Eu2 3_565 . 3_655 180 ?
Eu2 Eu2 Eu2 3_565 . 3_665 90.0000(11) ?
Eu2 Eu2 P1 3_565 . . 128.74(4) ?
Eu2 Eu2 P1 3_565 . 1_565 51.26(4) ?
Eu2 Eu2 P1 3_565 . 5_455 51.26(4) ?
Eu2 Eu2 P1 3_565 . 5_555 128.74(4) ?
Eu2 Eu2 Eu2 3_655 . 3_665 90.0000(11) ?
Eu2 Eu2 P1 3_655 . . 51.26(4) ?
Eu2 Eu2 P1 3_655 . 1_565 128.74(4) ?
Eu2 Eu2 P1 3_655 . 5_455 128.74(4) ?
Eu2 Eu2 P1 3_655 . 5_555 51.26(4) ?
Eu2 Eu2 P1 3_665 . . 128.74(4) ?
Eu2 Eu2 P1 3_665 . 1_565 51.26(4) ?
Eu2 Eu2 P1 3_665 . 5_455 128.74(4) ?
Eu2 Eu2 P1 3_665 . 5_555 51.26(4) ?
P1 Eu2 P1 . . 1_565 124.48(13) ?
P1 Eu2 P1 . . 5_455 102.53(5) ?
P1 Eu2 P1 . . 5_555 102.53(5) ?
P1 Eu2 P1 1_565 . 5_455 102.53(5) ?
P1 Eu2 P1 1_565 . 5_555 102.53(5) ?
P1 Eu2 P1 5_455 . 5_555 124.48(13) ?
Pt1 P1 Pt1 1_554 . . 180 ?
Pt1 P1 Pt2 1_554 . . 59.45(12) ?
Pt1 P1 Pt2 1_554 . 2_565 59.45(12) ?
Pt1 P1 Pt2 1_554 . 3_555 59.45(12) ?
Pt1 P1 Pt2 1_554 . 4_455 59.45(12) ?
Pt1 P1 Eu2 1_554 . 1_545 117.76(9) ?
Pt1 P1 Eu2 1_554 . . 117.76(9) ?
Pt1 P1 Eu2 1_554 . 3_555 117.76(9) ?
Pt1 P1 Eu2 1_554 . 3_655 117.76(9) ?
Pt1 P1 Pt2 . . . 120.55(12) ?
Pt1 P1 Pt2 . . 2_565 120.55(12) ?
Pt1 P1 Pt2 . . 3_555 120.55(12) ?
Pt1 P1 Pt2 . . 4_455 120.55(12) ?
Pt1 P1 Eu2 . . 1_545 62.24(9) ?
Pt1 P1 Eu2 . . . 62.24(9) ?
Pt1 P1 Eu2 . . 3_555 62.24(9) ?
Pt1 P1 Eu2 . . 3_655 62.24(9) ?
Pt2 P1 Pt2 . . 2_565 118.9(2) ?
Pt2 P1 Pt2 . . 3_555 75.03(11) ?
Pt2 P1 Pt2 . . 4_455 75.03(11) ?
Pt2 P1 Eu2 . . 1_545 72.41(2) ?
Pt2 P1 Eu2 . . . 140.860(8) ?
Pt2 P1 Eu2 . . 3_555 140.860(8) ?
Pt2 P1 Eu2 . . 3_655 72.41(2) ?
Pt2 P1 Pt2 2_565 . 3_555 75.03(11) ?
Pt2 P1 Pt2 2_565 . 4_455 75.03(11) ?
Pt2 P1 Eu2 2_565 . 1_545 140.860(8) ?
Pt2 P1 Eu2 2_565 . . 72.41(2) ?
Pt2 P1 Eu2 2_565 . 3_555 72.41(2) ?
Pt2 P1 Eu2 2_565 . 3_655 140.860(8) ?
Pt2 P1 Pt2 3_555 . 4_455 118.9(2) ?
Pt2 P1 Eu2 3_555 . 1_545 140.860(8) ?
Pt2 P1 Eu2 3_555 . . 72.41(2) ?
Pt2 P1 Eu2 3_555 . 3_555 140.860(8) ?
Pt2 P1 Eu2 3_555 . 3_655 72.41(2) ?
Pt2 P1 Eu2 4_455 . 1_545 72.41(2) ?
Pt2 P1 Eu2 4_455 . . 140.860(8) ?
Pt2 P1 Eu2 4_455 . 3_555 72.41(2) ?
Pt2 P1 Eu2 4_455 . 3_655 140.860(8) ?
Eu2 P1 Eu2 1_545 . . 124.48(18) ?
Eu2 P1 Eu2 1_545 . 3_555 77.47(7) ?
Eu2 P1 Eu2 1_545 . 3_655 77.47(7) ?
Eu2 P1 Eu2 . . 3_555 77.47(7) ?
Eu2 P1 Eu2 . . 3_655 77.47(7) ?
Eu2 P1 Eu2 3_555 . 3_655 124.48(18) ?

_exptl_crystal_preparation       'Magnetic properties'
####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_I_CCDC1
_database_code_depnum_ccdc_archive 'CCDC 1892355'
loop_
_audit_author_name
_audit_author_address
'Igor Plokhikh'
;University of Regensburg
Germany
;
_audit_update_record             
;
2019-01-21 deposited with the CCDC.	2019-09-23 downloaded from the CCDC.
;
#=======================================================================

# 5. CHEMICAL DATA

_chemical_name_systematic        'europium platinum phosphide'
_chemical_name_common            'europium platinum phosphide'
_chemical_formula_moiety         EuPt6P2
_chemical_formula_sum            'Eu Pt6 P2'
_chemical_compound_source        'solid state reaction'
_chemical_formula_structural     ?
_chemical_formula_analytical     ?
_chemical_formula_iupac          ?
_chemical_formula_weight         1384.4
_chemical_melting_point          ?
_exptl_crystal_description       powder
_exptl_crystal_colour            black

_diffrn_ambient_temperature      293
_diffrn_ambient_pressure         101.3

#=======================================================================

# 6. POWDER SPECIMEN AND CRYSTAL DATA

_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'P a -3'
_symmetry_Int_Tables_number      205
_chemical_absolute_configuration .
_symmetry_space_group_name_Hall  '-P 2ac;2ab;3'

loop_
_space_group_symop_id
_space_group_symop_operation_xyz
1 x,y,z
2 -x+1/2,-y,z+1/2
3 -x,y+1/2,-z+1/2
4 x+1/2,-y+1/2,-z
5 z,x,y
6 z+1/2,-x+1/2,-y
7 -z+1/2,-x,y+1/2
8 -z,x+1/2,-y+1/2
9 y,z,x
10 -y,z+1/2,-x+1/2
11 y+1/2,-z+1/2,-x
12 -y+1/2,-z,x+1/2
13 -x,-y,-z
14 x+1/2,y,-z+1/2
15 x,-y+1/2,z+1/2
16 -x+1/2,y+1/2,z
17 -z,-x,-y
18 -z+1/2,x+1/2,y
19 z+1/2,x,-y+1/2
20 z,-x+1/2,y+1/2
21 -y,-z,-x
22 y,-z+1/2,x+1/2
23 -y+1/2,z+1/2,x
24 y+1/2,z,-x+1/2

_cell_length_a                   8.46032(5)
_cell_length_b                   8.46032(5)
_cell_length_c                   8.46032(5)
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_volume                     605.564(6)


_cell_formula_units_Z            4
_cell_measurement_temperature    293
_cell_special_details            
; ?
;

_exptl_crystal_density_diffrn    15.1847
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_F_000             2244

_pd_spec_size_axial              ?
_pd_spec_size_equat              ?
_pd_spec_size_thick              ?
_pd_spec_mounting                ?
_pd_spec_mount_mode              ?
_pd_spec_shape                   ?
_pd_char_particle_morphology     ?
_pd_char_colour                  ?
_pd_prep_cool_rate               ?
_pd_prep_pressure                ?
_pd_prep_temperature             ?

_exptl_absorpt_coefficient_mu    149.537
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ?
_exptl_absorpt_correction_T_min  ?
_exptl_absorpt_correction_T_max  ?
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
? ? ? ?

#=======================================================================

# 7. EXPERIMENTAL DATA

_exptl_special_details           ?
_pd_instr_location               
; ?
;
_pd_calibration_special_details  
; ?
;

_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7093
_diffrn_source                   'sealed X-ray tube'
_diffrn_source_type              'STOE STADI P'
_diffrn_source_target            ?
_diffrn_radiation_monochromator  ?
_diffrn_measurement_device       'powder diffractometer'
_diffrn_measurement_device_type  'powder diffractometer'
_diffrn_detector                 ?
_diffrn_detector_type            ?

_pd_meas_scan_method             ?
_pd_meas_special_details         
; ?
;
_pd_meas_number_of_points        4262
_pd_meas_2theta_range_min        7.010
_pd_meas_2theta_range_max        70.925
_pd_meas_2theta_range_inc        0.015

#=======================================================================

# 8. REFINEMENT DATA

_pd_proc_ls_special_details      
; ?
;
_pd_proc_ls_profile_function     Pseudo-Voigt
_pd_proc_ls_background_function  '15 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_prof_R_factor        0.0193
_pd_proc_ls_prof_wR_factor       0.0259
_pd_proc_ls_prof_wR_expected     0.0181

_refine_special_details          
; ?
;

_refine_ls_R_factor_gt           0.0284
_refine_ls_wR_factor_gt          0.0238
_refine_ls_R_factor_all          0.0372
_refine_ls_wR_factor_all         0.0248
_refine_ls_goodness_of_fit_all   1.43
_refine_ls_restrained_S_gt       ?
_refine_ls_restrained_S_all      ?
_refine_ls_number_parameters     28
_refine_ls_number_restraints     0
_refine_ls_number_constraints    0
_refine_ls_weighting_scheme      sigma
_refine_ls_weighting_details     ?
_refine_ls_hydrogen_treatment    ?
_refine_ls_shift/su_max          0.0052
_refine_ls_shift/su_mean         0.0007
_refine_diff_density_max         3.68
_refine_diff_density_min         -4.79
_refine_ls_extinction_method     ?
_refine_ls_extinction_coef       ?
_refine_ls_extinction_expression ?

_pd_proc_2theta_range_min        7.01
_pd_proc_2theta_range_max        70.925
_pd_proc_2theta_range_inc        0.015
_pd_proc_wavelength              ?

_pd_block_diffractogram_id       ?

_pd_proc_info_excluded_regions   ?
_pd_proc_info_data_reduction     ?

loop_
_atom_type_symbol
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Eu -0.1003 3.6972 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
P 0.1037 0.0957 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'
Pt -1.6632 8.4516 'International Tables Vol C tables 4.2.6.8 and 6.1.1.1'

_computing_data_collection       ?
_computing_cell_refinement       ?
_computing_data_reduction        ?
_computing_structure_solution    ?
_computing_structure_refinement  ?
_computing_molecular_graphics    ?
_computing_publication_material  ?

loop_
_restr_distance_atom_site_label_1
_restr_distance_site_symmetry_1
_restr_distance_atom_site_label_2
_restr_distance_site_symmetry_2
_restr_distance_target
_restr_distance_target_weight_param
? ? ? ? ? ?


loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_adp_type
_atom_site_U_iso_or_equiv
_atom_site_site_symmetry_multiplicity
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_assembly
_atom_site_disorder_group
Pt1 Pt 0.65604(10) 0.34234(8) 0.07815(8) Uiso 0.00552(17) 24 1 d . . .
Eu1 Eu 0.5 0 0 Uiso 0.0072(5) 4 1 d . . .
P1 P 0.6956(6) 0.1956(6) 0.3044(6) Uiso 0.005(2) 8 1 d . . .

loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_1
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Pt1 Pt1 . 7_564 2.8118(10) ?
Pt1 Pt1 . 8_645 2.8274(11) ?
Pt1 Pt1 . 10_655 2.8118(10) ?
Pt1 Pt1 . 11_556 2.8274(11) ?
Pt1 Pt1 . 18_545 3.3773(10) ?
Pt1 Pt1 . 19_555 2.8160(11) ?
Pt1 Pt1 . 22_554 2.8160(11) ?
Pt1 Pt1 . 24_555 3.3773(10) ?
Pt1 Eu1 . . 3.2510(7) ?
Pt1 Eu1 . 3_655 4.0323(7) ?
Pt1 Eu1 . 4_555 3.2687(8) ?
Pt1 P1 . . 2.306(5) ?
Pt1 P1 . 15_554 2.362(5) ?
Eu1 P1 . . 3.480(5) ?
Eu1 P1 . 2_654 3.480(5) ?
Eu1 P1 . 3_645 3.480(5) ?
Eu1 P1 . 13_655 3.480(5) ?
Eu1 P1 . 14_455 3.480(5) ?
Eu1 P1 . 15_554 3.480(5) ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_2
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Pt1 Pt1 Pt1 7_564 . 8_645 137.05(3) ?
Pt1 Pt1 Pt1 7_564 . 10_655 60.00(3) ?
Pt1 Pt1 Pt1 7_564 . 11_556 162.94(4) ?
Pt1 Pt1 Pt1 7_564 . 18_545 93.35(3) ?
Pt1 Pt1 Pt1 7_564 . 19_555 90.00(3) ?
Pt1 Pt1 Pt1 7_564 . 22_554 60.05(3) ?
Pt1 Pt1 Pt1 7_564 . 24_555 85.17(3) ?
Pt1 Pt1 Eu1 7_564 . . 64.78(2) ?
Pt1 Pt1 Eu1 7_564 . 3_655 113.31(3) ?
Pt1 Pt1 Eu1 7_564 . 4_555 118.80(3) ?
Pt1 Pt1 P1 7_564 . . 133.94(12) ?
Pt1 Pt1 P1 7_564 . 15_554 53.47(12) ?
Pt1 Pt1 Pt1 8_645 . 10_655 124.01(4) ?
Pt1 Pt1 Pt1 8_645 . 11_556 60.00(3) ?
Pt1 Pt1 Pt1 8_645 . 18_545 92.81(3) ?
Pt1 Pt1 Pt1 8_645 . 19_555 130.90(4) ?
Pt1 Pt1 Pt1 8_645 . 22_554 145.80(4) ?
Pt1 Pt1 Pt1 8_645 . 24_555 53.09(2) ?
Pt1 Pt1 Eu1 8_645 . . 82.80(2) ?
Pt1 Pt1 Eu1 8_645 . 3_655 103.55(2) ?
Pt1 Pt1 Eu1 8_645 . 4_555 64.37(2) ?
Pt1 Pt1 P1 8_645 . . 52.19(12) ?
Pt1 Pt1 P1 8_645 . 15_554 92.56(12) ?
Pt1 Pt1 Pt1 10_655 . 11_556 112.89(3) ?
Pt1 Pt1 Pt1 10_655 . 18_545 143.16(3) ?
Pt1 Pt1 Pt1 10_655 . 19_555 60.05(3) ?
Pt1 Pt1 Pt1 10_655 . 22_554 90.00(3) ?
Pt1 Pt1 Pt1 10_655 . 24_555 93.09(3) ?
Pt1 Pt1 Eu1 10_655 . . 119.39(3) ?
Pt1 Pt1 Eu1 10_655 . 3_655 112.99(3) ?
Pt1 Pt1 Eu1 10_655 . 4_555 64.13(2) ?
Pt1 Pt1 P1 10_655 . . 165.07(12) ?
Pt1 Pt1 P1 10_655 . 15_554 53.47(12) ?
Pt1 Pt1 Pt1 11_556 . 18_545 84.93(3) ?
Pt1 Pt1 Pt1 11_556 . 19_555 73.52(3) ?
Pt1 Pt1 Pt1 11_556 . 22_554 106.41(3) ?
Pt1 Pt1 Pt1 11_556 . 24_555 111.34(3) ?
Pt1 Pt1 Eu1 11_556 . . 126.88(3) ?
Pt1 Pt1 Eu1 11_556 . 3_655 53.119(19) ?
Pt1 Pt1 Eu1 11_556 . 4_555 64.37(2) ?
Pt1 Pt1 P1 11_556 . . 52.19(12) ?
Pt1 Pt1 P1 11_556 . 15_554 137.16(12) ?
Pt1 Pt1 Pt1 18_545 . 19_555 98.31(3) ?
Pt1 Pt1 Pt1 18_545 . 22_554 53.40(2) ?
Pt1 Pt1 Pt1 18_545 . 24_555 110.68(3) ?
Pt1 Pt1 Eu1 18_545 . . 58.706(18) ?
Pt1 Pt1 Eu1 18_545 . 3_655 51.431(17) ?
Pt1 Pt1 Eu1 18_545 . 4_555 147.84(3) ?
Pt1 Pt1 P1 18_545 . . 44.32(12) ?
Pt1 Pt1 P1 18_545 . 15_554 131.96(12) ?
Pt1 Pt1 Pt1 19_555 . 22_554 59.90(3) ?
Pt1 Pt1 Pt1 19_555 . 24_555 150.82(3) ?
Pt1 Pt1 Eu1 19_555 . . 142.49(3) ?
Pt1 Pt1 Eu1 19_555 . 3_655 53.148(19) ?
Pt1 Pt1 Eu1 19_555 . 4_555 82.65(2) ?
Pt1 Pt1 P1 19_555 . . 110.07(12) ?
Pt1 Pt1 P1 19_555 . 15_554 113.30(12) ?
Pt1 Pt1 Pt1 22_554 . 24_555 137.32(3) ?
Pt1 Pt1 Eu1 22_554 . . 82.97(2) ?
Pt1 Pt1 Eu1 22_554 . 3_655 53.51(2) ?
Pt1 Pt1 Eu1 22_554 . 4_555 142.08(3) ?
Pt1 Pt1 P1 22_554 . . 94.08(12) ?
Pt1 Pt1 P1 22_554 . 15_554 113.30(12) ?
Pt1 Pt1 Eu1 24_555 . . 58.706(17) ?
Pt1 Pt1 Eu1 24_555 . 3_655 153.00(3) ?
Pt1 Pt1 Eu1 24_555 . 4_555 74.69(2) ?
Pt1 Pt1 P1 24_555 . . 93.61(12) ?
Pt1 Pt1 P1 24_555 . 15_554 43.00(12) ?
Eu1 Pt1 Eu1 . . 3_655 109.99(2) ?
Eu1 Pt1 Eu1 . . 4_555 133.15(2) ?
Eu1 Pt1 P1 . . . 75.41(12) ?
Eu1 Pt1 P1 . . 15_554 74.75(12) ?
Eu1 Pt1 Eu1 3_655 . 4_555 109.605(19) ?
Eu1 Pt1 P1 3_655 . . 59.40(12) ?
Eu1 Pt1 P1 3_655 . 15_554 163.58(12) ?
Eu1 Pt1 P1 4_555 . . 104.97(12) ?
Eu1 Pt1 P1 4_555 . 15_554 74.39(12) ?
P1 Pt1 P1 . . 15_554 136.07(17) ?
Pt1 Eu1 Pt1 . . 3_645 104.337(16) ?
Pt1 Eu1 Pt1 . . 4_455 92.242(19) ?
Pt1 Eu1 Pt1 . . 6_555 117.412(19) ?
Pt1 Eu1 Pt1 . . 7_564 51.096(18) ?
Pt1 Eu1 Pt1 . . 8_645 44.080(18) ?
Pt1 Eu1 Pt1 . . 9_554 99.587(18) ?
Pt1 Eu1 Pt1 . . 10_645 136.122(17) ?
Pt1 Eu1 Pt1 . . 12_554 117.412(19) ?
Pt1 Eu1 Pt1 . . 13_655 180 ?
Pt1 Eu1 Pt1 . . 15_554 75.663(16) ?
Pt1 Eu1 Pt1 . . 16_645 87.758(19) ?
Pt1 Eu1 Pt1 . . 18_545 62.588(19) ?
Pt1 Eu1 Pt1 . . 19_545 128.904(18) ?
Pt1 Eu1 Pt1 . . 20_554 135.920(18) ?
Pt1 Eu1 Pt1 . . 21_656 80.413(18) ?
Pt1 Eu1 Pt1 . . 22_554 43.878(17) ?
Pt1 Eu1 Pt1 . . 24_555 62.588(19) ?
Pt1 Eu1 P1 . . . 39.89(8) ?
Pt1 Eu1 P1 . . 2_654 102.70(8) ?
Pt1 Eu1 P1 . . 3_645 139.09(8) ?
Pt1 Eu1 P1 . . 13_655 140.11(8) ?
Pt1 Eu1 P1 . . 14_455 77.30(8) ?
Pt1 Eu1 P1 . . 15_554 40.91(8) ?
Pt1 Eu1 Pt1 3_645 . 4_455 91.292(17) ?
Pt1 Eu1 Pt1 3_645 . 6_555 136.122(17) ?
Pt1 Eu1 Pt1 3_645 . 7_564 126.116(16) ?
Pt1 Eu1 Pt1 3_645 . 8_645 96.044(15) ?
Pt1 Eu1 Pt1 3_645 . 9_554 136.161(17) ?
Pt1 Eu1 Pt1 3_645 . 10_645 96.044(15) ?
Pt1 Eu1 Pt1 3_645 . 12_554 44.080(18) ?
Pt1 Eu1 Pt1 3_645 . 13_655 75.663(16) ?
Pt1 Eu1 Pt1 3_645 . 15_554 180 ?
Pt1 Eu1 Pt1 3_645 . 16_645 88.708(17) ?
Pt1 Eu1 Pt1 3_645 . 18_545 43.878(17) ?
Pt1 Eu1 Pt1 3_645 . 19_545 53.884(16) ?
Pt1 Eu1 Pt1 3_645 . 20_554 83.956(15) ?
Pt1 Eu1 Pt1 3_645 . 21_656 43.839(17) ?
Pt1 Eu1 Pt1 3_645 . 22_554 83.956(15) ?
Pt1 Eu1 Pt1 3_645 . 24_555 135.920(18) ?
Pt1 Eu1 P1 3_645 . . 70.00(8) ?
Pt1 Eu1 P1 3_645 . 2_654 120.39(8) ?
Pt1 Eu1 P1 3_645 . 3_645 34.77(8) ?
Pt1 Eu1 P1 3_645 . 13_655 110.00(8) ?
Pt1 Eu1 P1 3_645 . 14_455 59.61(8) ?
Pt1 Eu1 P1 3_645 . 15_554 145.23(8) ?
Pt1 Eu1 Pt1 4_455 . 6_555 99.587(18) ?
Pt1 Eu1 Pt1 4_455 . 7_564 51.251(18) ?
Pt1 Eu1 Pt1 4_455 . 8_645 136.161(17) ?
Pt1 Eu1 Pt1 4_455 . 9_554 51.251(18) ?
Pt1 Eu1 Pt1 4_455 . 10_645 126.116(16) ?
Pt1 Eu1 Pt1 4_455 . 12_554 51.096(18) ?
Pt1 Eu1 Pt1 4_455 . 13_655 87.758(19) ?
Pt1 Eu1 Pt1 4_455 . 15_554 88.708(17) ?
Pt1 Eu1 Pt1 4_455 . 16_645 180 ?
Pt1 Eu1 Pt1 4_455 . 18_545 80.413(18) ?
Pt1 Eu1 Pt1 4_455 . 19_545 128.749(18) ?
Pt1 Eu1 Pt1 4_455 . 20_554 43.839(17) ?
Pt1 Eu1 Pt1 4_455 . 21_656 128.749(18) ?
Pt1 Eu1 Pt1 4_455 . 22_554 53.884(16) ?
Pt1 Eu1 Pt1 4_455 . 24_555 128.904(18) ?
Pt1 Eu1 P1 4_455 . . 112.27(8) ?
Pt1 Eu1 P1 4_455 . 2_654 139.17(8) ?
Pt1 Eu1 P1 4_455 . 3_645 88.56(8) ?
Pt1 Eu1 P1 4_455 . 13_655 67.73(8) ?
Pt1 Eu1 P1 4_455 . 14_455 40.83(8) ?
Pt1 Eu1 P1 4_455 . 15_554 91.44(8) ?
Pt1 Eu1 Pt1 6_555 . 7_564 92.242(19) ?
Pt1 Eu1 Pt1 6_555 . 8_645 104.337(16) ?
Pt1 Eu1 Pt1 6_555 . 9_554 51.096(18) ?
Pt1 Eu1 Pt1 6_555 . 10_645 44.080(18) ?
Pt1 Eu1 Pt1 6_555 . 12_554 117.412(19) ?
Pt1 Eu1 Pt1 6_555 . 13_655 62.588(19) ?
Pt1 Eu1 Pt1 6_555 . 15_554 43.878(17) ?
Pt1 Eu1 Pt1 6_555 . 16_645 80.413(18) ?
Pt1 Eu1 Pt1 6_555 . 18_545 180 ?
Pt1 Eu1 Pt1 6_555 . 19_545 87.758(19) ?
Pt1 Eu1 Pt1 6_555 . 20_554 75.663(16) ?
Pt1 Eu1 Pt1 6_555 . 21_656 128.904(18) ?
Pt1 Eu1 Pt1 6_555 . 22_554 135.920(18) ?
Pt1 Eu1 Pt1 6_555 . 24_555 62.588(19) ?
Pt1 Eu1 P1 6_555 . . 139.09(8) ?
Pt1 Eu1 P1 6_555 . 2_654 39.89(8) ?
Pt1 Eu1 P1 6_555 . 3_645 102.70(8) ?
Pt1 Eu1 P1 6_555 . 13_655 40.91(8) ?
Pt1 Eu1 P1 6_555 . 14_455 140.11(8) ?
Pt1 Eu1 P1 6_555 . 15_554 77.30(8) ?
Pt1 Eu1 Pt1 7_564 . 8_645 91.292(17) ?
Pt1 Eu1 Pt1 7_564 . 9_554 51.251(18) ?
Pt1 Eu1 Pt1 7_564 . 10_645 136.161(17) ?
Pt1 Eu1 Pt1 7_564 . 12_554 99.587(18) ?
Pt1 Eu1 Pt1 7_564 . 13_655 128.904(18) ?
Pt1 Eu1 Pt1 7_564 . 15_554 53.884(16) ?
Pt1 Eu1 Pt1 7_564 . 16_645 128.749(18) ?
Pt1 Eu1 Pt1 7_564 . 18_545 87.758(19) ?
Pt1 Eu1 Pt1 7_564 . 19_545 180 ?
Pt1 Eu1 Pt1 7_564 . 20_554 88.708(17) ?
Pt1 Eu1 Pt1 7_564 . 21_656 128.749(18) ?
Pt1 Eu1 Pt1 7_564 . 22_554 43.839(17) ?
Pt1 Eu1 Pt1 7_564 . 24_555 80.413(18) ?
Pt1 Eu1 P1 7_564 . . 88.56(8) ?
Pt1 Eu1 P1 7_564 . 2_654 112.27(8) ?
Pt1 Eu1 P1 7_564 . 3_645 139.17(8) ?
Pt1 Eu1 P1 7_564 . 13_655 91.44(8) ?
Pt1 Eu1 P1 7_564 . 14_455 67.73(8) ?
Pt1 Eu1 P1 7_564 . 15_554 40.83(8) ?
Pt1 Eu1 Pt1 8_645 . 9_554 126.116(16) ?
Pt1 Eu1 Pt1 8_645 . 10_645 96.044(15) ?
Pt1 Eu1 Pt1 8_645 . 12_554 136.122(17) ?
Pt1 Eu1 Pt1 8_645 . 13_655 135.920(18) ?
Pt1 Eu1 Pt1 8_645 . 15_554 83.956(15) ?
Pt1 Eu1 Pt1 8_645 . 16_645 43.839(17) ?
Pt1 Eu1 Pt1 8_645 . 18_545 75.663(16) ?
Pt1 Eu1 Pt1 8_645 . 19_545 88.708(17) ?
Pt1 Eu1 Pt1 8_645 . 20_554 180 ?
Pt1 Eu1 Pt1 8_645 . 21_656 53.884(16) ?
Pt1 Eu1 Pt1 8_645 . 22_554 83.956(15) ?
Pt1 Eu1 Pt1 8_645 . 24_555 43.878(17) ?
Pt1 Eu1 P1 8_645 . . 34.77(8) ?
Pt1 Eu1 P1 8_645 . 2_654 70.00(8) ?
Pt1 Eu1 P1 8_645 . 3_645 120.39(8) ?
Pt1 Eu1 P1 8_645 . 13_655 145.23(8) ?
Pt1 Eu1 P1 8_645 . 14_455 110.00(8) ?
Pt1 Eu1 P1 8_645 . 15_554 59.61(8) ?
Pt1 Eu1 Pt1 9_554 . 10_645 91.292(17) ?
Pt1 Eu1 Pt1 9_554 . 12_554 92.242(19) ?
Pt1 Eu1 Pt1 9_554 . 13_655 80.413(18) ?
Pt1 Eu1 Pt1 9_554 . 15_554 43.839(17) ?
Pt1 Eu1 Pt1 9_554 . 16_645 128.749(18) ?
Pt1 Eu1 Pt1 9_554 . 18_545 128.904(18) ?
Pt1 Eu1 Pt1 9_554 . 19_545 128.749(18) ?
Pt1 Eu1 Pt1 9_554 . 20_554 53.884(16) ?
Pt1 Eu1 Pt1 9_554 . 21_656 180 ?
Pt1 Eu1 Pt1 9_554 . 22_554 88.708(17) ?
Pt1 Eu1 Pt1 9_554 . 24_555 87.758(19) ?
Pt1 Eu1 P1 9_554 . . 139.17(8) ?
Pt1 Eu1 P1 9_554 . 2_654 88.56(8) ?
Pt1 Eu1 P1 9_554 . 3_645 112.27(8) ?
Pt1 Eu1 P1 9_554 . 13_655 40.83(8) ?
Pt1 Eu1 P1 9_554 . 14_455 91.44(8) ?
Pt1 Eu1 P1 9_554 . 15_554 67.73(8) ?
Pt1 Eu1 Pt1 10_645 . 12_554 104.337(16) ?
Pt1 Eu1 Pt1 10_645 . 13_655 43.878(17) ?
Pt1 Eu1 Pt1 10_645 . 15_554 83.956(15) ?
Pt1 Eu1 Pt1 10_645 . 16_645 53.884(16) ?
Pt1 Eu1 Pt1 10_645 . 18_545 135.920(18) ?
Pt1 Eu1 Pt1 10_645 . 19_545 43.839(17) ?
Pt1 Eu1 Pt1 10_645 . 20_554 83.956(15) ?
Pt1 Eu1 Pt1 10_645 . 21_656 88.708(17) ?
Pt1 Eu1 Pt1 10_645 . 22_554 180 ?
Pt1 Eu1 Pt1 10_645 . 24_555 75.663(16) ?
Pt1 Eu1 P1 10_645 . . 120.39(8) ?
Pt1 Eu1 P1 10_645 . 2_654 34.77(8) ?
Pt1 Eu1 P1 10_645 . 3_645 70.00(8) ?
Pt1 Eu1 P1 10_645 . 13_655 59.61(8) ?
Pt1 Eu1 P1 10_645 . 14_455 145.23(8) ?
Pt1 Eu1 P1 10_645 . 15_554 110.00(8) ?
Pt1 Eu1 Pt1 12_554 . 13_655 62.588(19) ?
Pt1 Eu1 Pt1 12_554 . 15_554 135.920(18) ?
Pt1 Eu1 Pt1 12_554 . 16_645 128.904(18) ?
Pt1 Eu1 Pt1 12_554 . 18_545 62.588(19) ?
Pt1 Eu1 Pt1 12_554 . 19_545 80.413(18) ?
Pt1 Eu1 Pt1 12_554 . 20_554 43.878(17) ?
Pt1 Eu1 Pt1 12_554 . 21_656 87.758(19) ?
Pt1 Eu1 Pt1 12_554 . 22_554 75.663(16) ?
Pt1 Eu1 Pt1 12_554 . 24_555 180 ?
Pt1 Eu1 P1 12_554 . . 102.70(8) ?
Pt1 Eu1 P1 12_554 . 2_654 139.09(8) ?
Pt1 Eu1 P1 12_554 . 3_645 39.89(8) ?
Pt1 Eu1 P1 12_554 . 13_655 77.30(8) ?
Pt1 Eu1 P1 12_554 . 14_455 40.91(8) ?
Pt1 Eu1 P1 12_554 . 15_554 140.11(8) ?
Pt1 Eu1 Pt1 13_655 . 15_554 104.337(16) ?
Pt1 Eu1 Pt1 13_655 . 16_645 92.242(19) ?
Pt1 Eu1 Pt1 13_655 . 18_545 117.412(19) ?
Pt1 Eu1 Pt1 13_655 . 19_545 51.096(18) ?
Pt1 Eu1 Pt1 13_655 . 20_554 44.080(18) ?
Pt1 Eu1 Pt1 13_655 . 21_656 99.587(18) ?
Pt1 Eu1 Pt1 13_655 . 22_554 136.122(17) ?
Pt1 Eu1 Pt1 13_655 . 24_555 117.412(19) ?
Pt1 Eu1 P1 13_655 . . 140.11(8) ?
Pt1 Eu1 P1 13_655 . 2_654 77.30(8) ?
Pt1 Eu1 P1 13_655 . 3_645 40.91(8) ?
Pt1 Eu1 P1 13_655 . 13_655 39.89(8) ?
Pt1 Eu1 P1 13_655 . 14_455 102.70(8) ?
Pt1 Eu1 P1 13_655 . 15_554 139.09(8) ?
Pt1 Eu1 Pt1 15_554 . 16_645 91.292(17) ?
Pt1 Eu1 Pt1 15_554 . 18_545 136.122(17) ?
Pt1 Eu1 Pt1 15_554 . 19_545 126.116(16) ?
Pt1 Eu1 Pt1 15_554 . 20_554 96.044(15) ?
Pt1 Eu1 Pt1 15_554 . 21_656 136.161(17) ?
Pt1 Eu1 Pt1 15_554 . 22_554 96.044(15) ?
Pt1 Eu1 Pt1 15_554 . 24_555 44.080(18) ?
Pt1 Eu1 P1 15_554 . . 110.00(8) ?
Pt1 Eu1 P1 15_554 . 2_654 59.61(8) ?
Pt1 Eu1 P1 15_554 . 3_645 145.23(8) ?
Pt1 Eu1 P1 15_554 . 13_655 70.00(8) ?
Pt1 Eu1 P1 15_554 . 14_455 120.39(8) ?
Pt1 Eu1 P1 15_554 . 15_554 34.77(8) ?
Pt1 Eu1 Pt1 16_645 . 18_545 99.587(18) ?
Pt1 Eu1 Pt1 16_645 . 19_545 51.251(18) ?
Pt1 Eu1 Pt1 16_645 . 20_554 136.161(17) ?
Pt1 Eu1 Pt1 16_645 . 21_656 51.251(18) ?
Pt1 Eu1 Pt1 16_645 . 22_554 126.116(16) ?
Pt1 Eu1 Pt1 16_645 . 24_555 51.096(18) ?
Pt1 Eu1 P1 16_645 . . 67.73(8) ?
Pt1 Eu1 P1 16_645 . 2_654 40.83(8) ?
Pt1 Eu1 P1 16_645 . 3_645 91.44(8) ?
Pt1 Eu1 P1 16_645 . 13_655 112.27(8) ?
Pt1 Eu1 P1 16_645 . 14_455 139.17(8) ?
Pt1 Eu1 P1 16_645 . 15_554 88.56(8) ?
Pt1 Eu1 Pt1 18_545 . 19_545 92.242(19) ?
Pt1 Eu1 Pt1 18_545 . 20_554 104.337(16) ?
Pt1 Eu1 Pt1 18_545 . 21_656 51.096(18) ?
Pt1 Eu1 Pt1 18_545 . 22_554 44.080(18) ?
Pt1 Eu1 Pt1 18_545 . 24_555 117.412(19) ?
Pt1 Eu1 P1 18_545 . . 40.91(8) ?
Pt1 Eu1 P1 18_545 . 2_654 140.11(8) ?
Pt1 Eu1 P1 18_545 . 3_645 77.30(8) ?
Pt1 Eu1 P1 18_545 . 13_655 139.09(8) ?
Pt1 Eu1 P1 18_545 . 14_455 39.89(8) ?
Pt1 Eu1 P1 18_545 . 15_554 102.70(8) ?
Pt1 Eu1 Pt1 19_545 . 20_554 91.292(17) ?
Pt1 Eu1 Pt1 19_545 . 21_656 51.251(18) ?
Pt1 Eu1 Pt1 19_545 . 22_554 136.161(17) ?
Pt1 Eu1 Pt1 19_545 . 24_555 99.587(18) ?
Pt1 Eu1 P1 19_545 . . 91.44(8) ?
Pt1 Eu1 P1 19_545 . 2_654 67.73(8) ?
Pt1 Eu1 P1 19_545 . 3_645 40.83(8) ?
Pt1 Eu1 P1 19_545 . 13_655 88.56(8) ?
Pt1 Eu1 P1 19_545 . 14_455 112.27(8) ?
Pt1 Eu1 P1 19_545 . 15_554 139.17(8) ?
Pt1 Eu1 Pt1 20_554 . 21_656 126.116(16) ?
Pt1 Eu1 Pt1 20_554 . 22_554 96.044(15) ?
Pt1 Eu1 Pt1 20_554 . 24_555 136.122(17) ?
Pt1 Eu1 P1 20_554 . . 145.23(8) ?
Pt1 Eu1 P1 20_554 . 2_654 110.00(8) ?
Pt1 Eu1 P1 20_554 . 3_645 59.61(8) ?
Pt1 Eu1 P1 20_554 . 13_655 34.77(8) ?
Pt1 Eu1 P1 20_554 . 14_455 70.00(8) ?
Pt1 Eu1 P1 20_554 . 15_554 120.39(8) ?
Pt1 Eu1 Pt1 21_656 . 22_554 91.292(17) ?
Pt1 Eu1 Pt1 21_656 . 24_555 92.242(19) ?
Pt1 Eu1 P1 21_656 . . 40.83(8) ?
Pt1 Eu1 P1 21_656 . 2_654 91.44(8) ?
Pt1 Eu1 P1 21_656 . 3_645 67.73(8) ?
Pt1 Eu1 P1 21_656 . 13_655 139.17(8) ?
Pt1 Eu1 P1 21_656 . 14_455 88.56(8) ?
Pt1 Eu1 P1 21_656 . 15_554 112.27(8) ?
Pt1 Eu1 Pt1 22_554 . 24_555 104.337(16) ?
Pt1 Eu1 P1 22_554 . . 59.61(8) ?
Pt1 Eu1 P1 22_554 . 2_654 145.23(8) ?
Pt1 Eu1 P1 22_554 . 3_645 110.00(8) ?
Pt1 Eu1 P1 22_554 . 13_655 120.39(8) ?
Pt1 Eu1 P1 22_554 . 14_455 34.77(8) ?
Pt1 Eu1 P1 22_554 . 15_554 70.00(8) ?
Pt1 Eu1 P1 24_555 . . 77.30(8) ?
Pt1 Eu1 P1 24_555 . 2_654 40.91(8) ?
Pt1 Eu1 P1 24_555 . 3_645 140.11(8) ?
Pt1 Eu1 P1 24_555 . 13_655 102.70(8) ?
Pt1 Eu1 P1 24_555 . 14_455 139.09(8) ?
Pt1 Eu1 P1 24_555 . 15_554 39.89(8) ?
P1 Eu1 P1 . . 2_654 103.07(11) ?
P1 Eu1 P1 . . 3_645 103.07(11) ?
P1 Eu1 P1 . . 13_655 180 ?
P1 Eu1 P1 . . 14_455 76.93(11) ?
P1 Eu1 P1 . . 15_554 76.93(11) ?
P1 Eu1 P1 2_654 . 3_645 103.07(11) ?
P1 Eu1 P1 2_654 . 13_655 76.93(11) ?
P1 Eu1 P1 2_654 . 14_455 180 ?
P1 Eu1 P1 2_654 . 15_554 76.93(11) ?
P1 Eu1 P1 3_645 . 13_655 76.93(11) ?
P1 Eu1 P1 3_645 . 14_455 76.93(11) ?
P1 Eu1 P1 3_645 . 15_554 180 ?
P1 Eu1 P1 13_655 . 14_455 103.07(11) ?
P1 Eu1 P1 13_655 . 15_554 103.07(11) ?
P1 Eu1 P1 14_455 . 15_554 103.07(11) ?
Pt1 P1 Pt1 . . 8_645 75.63(15) ?
Pt1 P1 Pt1 . . 11_556 75.63(15) ?
Pt1 P1 Pt1 . . 15_555 150.1(2) ?
Pt1 P1 Pt1 . . 18_545 92.68(17) ?
Pt1 P1 Pt1 . . 21_656 128.7(2) ?
Pt1 P1 Eu1 . . . 64.70(11) ?
Pt1 P1 Eu1 . . 2_655 139.31(18) ?
Pt1 P1 Eu1 . . 3_655 85.83(14) ?
Pt1 P1 Pt1 8_645 . 11_556 75.63(15) ?
Pt1 P1 Pt1 8_645 . 15_555 128.7(2) ?
Pt1 P1 Pt1 8_645 . 18_545 150.1(2) ?
Pt1 P1 Pt1 8_645 . 21_656 92.68(17) ?
Pt1 P1 Eu1 8_645 . . 85.83(14) ?
Pt1 P1 Eu1 8_645 . 2_655 64.70(11) ?
Pt1 P1 Eu1 8_645 . 3_655 139.31(18) ?
Pt1 P1 Pt1 11_556 . 15_555 92.68(17) ?
Pt1 P1 Pt1 11_556 . 18_545 128.7(2) ?
Pt1 P1 Pt1 11_556 . 21_656 150.1(2) ?
Pt1 P1 Eu1 11_556 . . 139.31(18) ?
Pt1 P1 Eu1 11_556 . 2_655 85.83(14) ?
Pt1 P1 Eu1 11_556 . 3_655 64.70(11) ?
Pt1 P1 Pt1 15_555 . 18_545 73.05(14) ?
Pt1 P1 Pt1 15_555 . 21_656 73.05(14) ?
Pt1 P1 Eu1 15_555 . . 126.41(17) ?
Pt1 P1 Eu1 15_555 . 2_655 64.78(11) ?
Pt1 P1 Eu1 15_555 . 3_655 64.33(11) ?
Pt1 P1 Pt1 18_545 . 21_656 73.05(14) ?
Pt1 P1 Eu1 18_545 . . 64.33(11) ?
Pt1 P1 Eu1 18_545 . 2_655 126.41(17) ?
Pt1 P1 Eu1 18_545 . 3_655 64.78(11) ?
Pt1 P1 Eu1 21_656 . . 64.78(11) ?
Pt1 P1 Eu1 21_656 . 2_655 64.33(11) ?
Pt1 P1 Eu1 21_656 . 3_655 126.41(17) ?
Eu1 P1 Eu1 . . 2_655 118.54(13) ?
Eu1 P1 Eu1 . . 3_655 118.54(13) ?
Eu1 P1 Eu1 2_655 . 3_655 118.54(13) ?
